Title: Novel Dry Metal Electrode with Tilted MicrostructureFabricated with Laser Micromilling Process
Authors: Wei Zhou, Shaoyu Liu, Wei Liu, Chenying Zhang,Yaoyao Li, Wenjing Xu, Kwan San Hui
PII: S0924-4247(17)30319-9DOI: http://dx.doi.org/doi:10.1016/j.sna.2017.07.028Reference: SNA 10223
To appear in: Sensors and Actuators A
Received date: 22-2-2017Revised date: 12-7-2017Accepted date: 13-7-2017
Please cite this article as: Wei Zhou, Shaoyu Liu, Wei Liu, Chenying Zhang,Yaoyao Li, Wenjing Xu, Kwan San Hui, Novel Dry Metal Electrode with TiltedMicrostructure Fabricated with Laser Micromilling Process, Sensors and Actuators:A Physicalhttp://dx.doi.org/10.1016/j.sna.2017.07.028
This is a PDF file of an unedited manuscript that has been accepted for publication.As a service to our customers we are providing this early version of the manuscript.The manuscript will undergo copyediting, typesetting, and review of the resulting proofbefore it is published in its final form. Please note that during the production processerrors may be discovered which could affect the content, and all legal disclaimers thatapply to the journal pertain.
Page 1 of 21
Novel Dry Metal Electrode with Tilted Microstructure
Fabricated with Laser Micromilling Process
Wei Zhou a *, Shaoyu Liu a, Wei Liua, Chenying Zhang a, Yaoyao Li a,
Wenjing Xu a, Kwan San Hui b
a Department of Mechanical & Electrical Engineering, Xiamen University, Xiamen
b School of Mathematics, University of East Anglia, Norwich, NR4 7TJ, United
> Dry metal electrodes with tilted microstructure arrays is fabricated. > Laser
micromilling process of tilted microstructure arrays is discussed. > Effect of process
parameters on surface microstructure arrays is investigated. > Optimized process
parameters are obtained to fabricate tilted microstructure arrays. > Eelectrodes with
tilted microstructures show lower impedance than vertical microstructures.
Abstract: A novel dry metal electrodes with tilted microstructure arrays was fabricated
with laser micromilling process by adjusting the incident angle of the laser beam. After
discussing the laser fabrication process for dry metal electrodes, the effects of the laser
incident angle, width of unscanned area, laser output power, and scanning times on the
shape and size of the microstructures are further discussed. Our experimental results
show that the tilted angle of the surface microstructures of the dry metal electrodes
depended on the laser incident angle. The heights of the surface microstructures of dry
metal electrodes were greatly increased by increases of the laser output power and
scanning times. Compared with vertical microstructure arrays, the developed dry metal
electrodes with 60° tilted angle microstructure arrays demonstrated much lower
Page 2 of 21
Keywords: Dry metal electrode; Laser micromilling; Surface microstructures;
*Corresponding author. Tel.: 86-592-2188698; Fax: 86-592-2186383
[email protected] (Wei Zhou).
Over the last decade, the research on and applications of bioelectrical signals has
been given increasing attention with the rapid development of modern medicine,
neurology, and artificial intelligence. Bioelectrodes, which can be used to measure
biological signals, have been widely used in modern clinical and biomedical
measurements, including electrocardiograph (ECG), electroencephalogram (EEG),
electromyography (EMG), gastric electrical activity, nerve potential, and electrical
impedance imaging (EIT) measurements . In the detecting process of biological
electrical signals, a bioelectrode system, as a significant component of the measurement
system, will come into direct contact with human skin, input a drive current, and receive
a voltage signal for the purpose of exchanging and transmitting information. Because
of the weak strengths of bioelectrical signals, there are strict conductivity requirements
for bioelectrodes, which commonly use metal, silicon, or polymer as the base materials,
covered by a conductive metal layer on the surface. Moreover, bioelectrodes, which
come into direct contact with human skin, should be non-toxic and cannot cause allergic
reactions . Several bioelectrodes have been developed to meet the requirements for
biological electrical signals measurement. Based on the structure style, bioelectrodes
are divided into the traditional Ag/AgCl wet electrode, microneedle electrode, flexible
Page 3 of 21
textile electrode, foam electrode and insulated dry electrode.
To fabricate the microstructure electrodes, the micromachining technology has been
developed to fabricate microstructure arrays on silicon, metal, polymer, and glass,
where the size of a single microstructure is usually 30–80 µm, with a length of more
than 100 µm. Although most of the research has focused on an etching process to form
microstructures on silicon [3–5], some researchers have developed some fabrication
methods,such as traditional machining, electrochemical machining and 3D printing
using the metal or other materials [6–13]. Ng et al.  developed a vacuum casting
method to fabricate micro-spike dry EEG electrodes. These electrodes, which had a low
impedance and stable performance, showed a good EEG measurement ability. Salvo et
al.  developed a 3D printing method to fabricate a microneedle electrode, which was
applied to EEG and ECG measurements and had a better performance than the
traditional wet electrodes. Ruffini et al.  developed a novel electrode formed by
carbon nanotubes. Because of its good ability to adhere to the surface of human skin,
this electrode showed an accurate bioelectrical signal performance. Kitamura et al. [9-
10] proposed an electrolytical method to fabricate electrodes using the steel wire. This
method was simple, saved time, and allowed the shape of the microneedle structure to
be controlled. Electrodes fabricated using this method had good performances as the
traditional Ag/AgCl wet electrodes. Recently, seveal papers reported their work in
developing novel dry electrodes with laser method. Laser processing, which is fast and
accurate, has outstanding advantages in fabricating the microstructure[14-15]. For
example, Gill et al.  developed a new method to fabricate miconeedle electrode, the
Page 4 of 21
laser beam ablated the metal sheet and created the miconeedles in the plane of the sheet,
then miconeedles was manually bent at 90° and electropolished, and the sizes and
shapes of this electrodes can be controlled.
In this study, we proposed a laser micromilling fabrication method to make novel dry
metal electrodes, which allows tilted microstructure arrays to be formed on the surface
of the dry electrode by adjusting the incident angle of the laser beam. Based on the
principle of the laser machining method, the effects of laser incident angle, width of
unscanned area, laser output power, and scanning times on the shape and size of the
microstructure were discussed in detail. Finally, impedance measurement of dry metal
electrodes with tilted microstructure arrays was conducted and compared with vertical
2 Design, fabrication and impedance measurement of dry metal
2.1 Structural design of dry metal electrode
A schematic diagram of a dry metal electrode with tilted microstructure array is
shown in Fig.1. The metal dry electrode was composed of a metal electrode core,
medical gauze, conductive silver glue, foam backing material, and shielding wire. The
metal electrode core was made of red copper, which had good machinability and
conductivity . Laser micromilling was employed to fabricate the 6×6
microstructure arrays on the surface of metal electrode core with the size of 8×8 mm2.
After the laser micromilling process, platinum was sputtered on the core to improve the
contact between the electrode core and human skin, which cloud improves the accuracy
Page 5 of 21
of the biological electrical signal measurement. Moreover, a shielding wire was stuck
to the metal electrode core using conductive silver glue and covered by a foam backing
material. Then, the medical gauze was affixed to the back side, and the dry metal
electrode was finally assembled. These surface microstructures are beneficial to
improve the contact interface and increase the friction force between the electrode and
skin, leading to a low contact impedance and better measurement stability.
2.2 Laser micromilling process
Fig. 2. shows the schematic diagram of the experimental setup for the laser
micromilling process used for the dry metal bioelectrode. The system was composed of
a fiber laser, collimator head, F-theta objective lens, computer controller, and
machining platform . In this study, a pulsed fiber laser (IPG) was used . The laser
was set to produce 100 ns pulses with a 1064 nm central emission wavelength at a
repetition rate of 20 kHz. The specifications of the characteristic parameters of the fiber
laser system used are given in Table 1. The machining platform was composed of
a linear motion device, rotating device, and fixture. The linear motion device was driven
by a small stepper motor, which generated a reciprocating motion on the Z axis. A hinge
was used to connect the linear motion device and rotating device, and the rotating
device could rotate around the Y axis. The fixture was used to fix a copper plate. The
incident angle of the laser beam could be controlled by changing the angle of the
machining platform. In addition, laser processing parameters such as the unscanning
area, laser output power, and scanning time could be adjusted through computer control.
One significant parameter of laser milling is the energy density (ED), which is
Page 6 of 21
determined as follows:
where PA is the output power of the laser source at a fixed frequency, Vscan is the
scanning speed, and фspot is the focused diameter of the laser spot [19–21].
In this study, the threshold value of about 0.35 J/cm2 can be experimentally derived
for red copper matrial.When the laser output power was selected over 20 W and
scanning speed below 1000mm/s, the red copper substrate can be fabricated.
2.3 Impedance measurement step
Fig. 3. shows the schematic diagram of impedance measurement of dry metal
electrode. Two dry metal electrodes were placed on the forearm to measure the
electrode–skin impedance, with a distance between the electrodes of 5 cm [22–23]. The
dry metal electrodes did not require any treatment of the skin before the measurement
[24–26]. Based on the two-electrode measurement principle, the same pair of electrodes
could be used for the driving and measurement electrodes. The impedance analyzer
(HIOKI Im3523 LCR Meter, Japan) was controlled by the Labview program through a
USB interface. The computer sent a signal at a specific frequency to the impedance
analyzer, which generated a sinusoidal current of 1 mA. Then, the impedance analyzer
sent the current to the two electrodes on the forearm and measured their potentials.
Finally, the impedance analyzer transmitted the impedance data to the computer
through the USB interface, and the data was recorded and analyzed by Labview
software. A frequency of 50 kHz was used by the impedance analyzer, and the working
mode was the Z-R mode [27-28]. Short circuit and open circuit calibrations were
Page 7 of 21
performed to improve the measurement accuracy before the impedance data was
3 Results and discussion
3.1 Formation process of tilted microstructure array
Laser processing is a thermal processing based on the photothermal effect. When
a pulsed laser irradiates the base metal, it absorbs the laser beam energy, which causes
the temperature of the metal to rapidly rise and exceed the evaporation temperature.
The metal around the laser spot then melts even vaporizes at the high temperature,
leading to material removal. The vaporized material will continue to interact with the
laser beam, with some of the material becoming ionized and forming a plasma, which
affect the further absorption of laser energy. Recasting is a normal phenomenon in the
laser micromachining process. This phenomenon causes materials to transfer from the
area that has been scanned by the laser to the area that has not been scanned . With
the help of this phenomenon, the recast layer stacking process can be controlled to form
a microstructure array on the surface of the dry metal electrode.
As shown in Fig. 4a. to fabricate a dry metal electrode with a tilted microstructure
array, the nested square machining path and loop multiple-pass reciprocating scanning
strategies were used in this study. Fig. 4b. shows the schematic diagram of machining
platform used to fabricate the dry metal electrodes. The incident angle (θ) of the laser
beam directly affects the angle of the microstructures on the surface of the dry metal
electrode. Fig. 4c. shows the effect of using a small scanning process for the substrate.
As a result of gravity, the amount of recast metal below the molten pool was greater
Page 8 of 21
than that above it. As the number of scans gradually increases, the laser energy is
absorbed by the continuous irradiation of the laser. At this stage, the unscanned area
was continually covered by the recast metal, as shown in Fig. 4d. Later, as the number
of scans increases, a greater amount of surface material is heated to produce the metal
steam pressure, which causes further external ejection of the liquid material to increase
the depth and width of the scanning area, and a large quantity of metal is effectively
removed during the laser micromilling process . Finally, the recast metal is
deposited and integrated with the unscanned area to form the cone microstructure array
on the surface of the sample metal [30-31], as shown in Fig. 4e. Fig. 5. shows a typical
scanning electron microscope (SEM) image of a tilted microstructure array on the
surface of a dry metal electrode. It was verified that a tilted microstructure electrode
could be successfully fabricated by controlling the incident angle of the laser beam.
3.2 Effects of process parameters on tilted microstructure array
3.2.1 Laser incident angle
Fig. 6. shows SEM images of dry metal electrodes with tilted microstructure
arrays fabricated with different laser incident angles. The incident angle was set at
60°–90° by controlling the angle of the machining platform. The other machining
parameters were fixed at a laser output power of 27 W, a scanning speed of 500 mm/s,
30 scanning times, and an unscanned area width of 100 μm. When the incident angle
changes from 60° to 90°, the shape of the microstructures changes from a tilted style
to a vertical style. Table 2 lists the measurement data of the tilted angle and height of
microstructures fabricated with different laser incident angles. It can be observed from
Page 9 of 21
the table that the error between the tilted angle of the microstructures and laser
incident angle was within 2°. Furthermore, the height of the microstructures is also
affected by the laser incident angle. When the laser incident angle was 60°, the height
was found to reach a maximum value of 496 μm. However, the microstructure array
could not be fabricated with a small laser incident angle. Therefore, we recommend
60° laser incident angle to produce the microstructure array on the surface of dry
metal electrodes with much better quality.
3.2.2 Width of unscanned area
The machining path is one of the most important parameters influencing the laser
micromilling process. In this experiment, a nested square machining path was
selected, and the inner square was the unscanned area, as shown in Fig. 4. Widths of
60 µm, 80 µm, 100 µm, and 120 µm were selected for the unscanned area under the
predetermined conditions of a laser output power of 27 W, a scanning speed of 500
mm/s, 30 scanning times, and a 60° laser incident angle. When the width was set at 60
µm, it was obvious that an microstructure array was formed on the surface of the
sample metal, as shown in Fig. 7a. This was mainly because the small unscanned area
led to a small area for recasting, but the small recast area could not hold most of the
molten and vaporized metal. When the width was increased to 120 µm, the unscanned
area was too large to be covered by the recast metal, which led to ladder structures.
However, when a width of 80–100 µm was selected, the cone microstructure arrays
were formed, which means the recast metal exactly covered the unscanned area, as
shown in Fig. 7b. and c.
Page 10 of 21
Fig. 8. shows the influence of the unscanned area width on the height and bottom
width of tilted microstructurethe of dry metal electrode. It can be seen that the width
of the unscanned area has a significant influence on the bottom width of the
microstructures. When the width of the unscanned area was increased from 60 μm to
120 μm, the bottom width of the microstructures increased from 151 µm to 379 µm.
The height of the microstructures gradually increases when the width of the
unscanned area increases from 60 μm to 100 μm, but when the width increases to 120
μm, the height decreases. These changes were attributed to the difficulty of covering a
large unscanned area with the recast metal material and the fact that a small
unscanned area could not hold most of the recast metal material. Thus, in both cases,
the cone microstructure array could not be formed. Therefore, 80–100 µm was the
optimized width for the unscanned area.
3.2.3 Laser output power
The laser output power is one of the significant parameters in the micromilling
process. Laser output power values of 21 W, 24 W, 27 W, and 30 W were selected
under the predetermined conditions of a scanning speed of 500 mm/s, 30 scanning
times, an unscanned area width of 100 μm, and a 60° laser incident angle. The effects
of the laser output power on the shape and size of the microstructures were studied
based on the SEM images. When the laser output power was 21 W, the surface
microstructures could not be effectively fabricated because the low laser energy made
it difficult to fully achieve the surface evaporation and melting process of the surface
metal material, which led to a low material removal rate, as shown in Fig. 9a.
Page 11 of 21
However, when the laser output power was increased to more than 24 W, the material
melting and evaporation phenomena become much easier to induce because of the
higher temperature. Finally, the surface material was removed to produce the
surface microstructures, as shown in Fig. 9b. to d. The influence of the laser output
power on height and bottom width of tilted microstructures of dry metal electrode is
shown in Fig.10. When the laser output power was increased from 21 W to 30 W, the
bottom width increases from 229 µm to 359 µm, and the height increases from 248
µm to 480 µm. It is worth noting that the laser output power has a greater influence on
the height of the microstructures than on the bottom width. This was attributed to the
fact that the influence of the laser output power on the depth of the melting zone was
greater than that on the width.
3.2.4 Scanning times
The scanning times, which determined the quality of the structure, also needed to
be adjusted in the laser micromilling process. SEM images of tilted microstructures
produced using different scanning times are shown in Fig. 11. Where the
predetermined conditions were a laser output power value of 27 W, a scanning speed
of 500 mm/s, an unscanned area width of 100 μm, and a laser incident angle of 60°.
When the scanning times were less than 10 times, it was difficult to form the top of
the microstructures, and the total height was low, as a result of the low material
removal rate, as shown in Fig. 11a. When the scanning times were increased to 20
times, the cone microstructure array were gradually formed, as shown in Fig. 11b.
Finally, when more than 30 scanning times were used, the cone microstructure array
Page 12 of 21
were successfully fabricated, as shown in Fig. 11c. and d. However, the scanning
times had a greater effect on the height of the microstructures than on their width,
which can be seen in Fig. 12. When the scanning times were increased from 10 times
to 50 times, the height of the microstructures increased from 126 µm to 480 µm,
whereas the width increased from 160 µm to 314 µm. Therefore, to obtain dry metal
electrodes with a tilted surface microstructure array, the scan times should be greater
3.3 Impedance measurement
Fig. 13. shows the impedance measured value using dry metal electrodes with
different tilted degree microstructure array and without microstructure array. Under the
same measurement conditions, the dry metal electrodes with tilted degree
microstructure array had lower average impedance values comparing with the
electrodes without microstructure array. Furthermore, the dry metal electrodes with the
60° tilted microstructure array had lower average impedance values than those with the
vertical microstructures (less about 18 Ω), as show in Fig. 13a. Fig. 13b. shows the
impedance measurements over a period of 20 min. The impedance measured by the dry
metal electrodes with 60° tilted microstructures presented small fluctuations in the first
15 min, and then gradually became stable, reaching a value that was lower than that of
the electrodes with the vertical microstructures (90°). This can be attributed to the fact
that the dry metal electrodes with the tilted microstructures fit more tightly than those
with the vertical microstructures. However, the tilted microstructures may have needed
more time to become joined to the skin, which led to a slightly longer settling time.
Page 13 of 21
Therefore, the dry metal electrodes with the tilted microstructures have an advantage in
long-term impedance measurement compared with those with vertical microstructures.
Tilted microstructure arrays could be fabricated with laser micromilling process on
the surface of dry metal electrodes by adjusting the incident angle of the laser beam.
The influence of the laser incident angle, unscanning area width, laser output power
and scanning times on the formation of the microstructure was discussed. In the laser
micromilling process, the tilted angle of the surface microstructures of the dry metal
electrodes depended on the laser incident angle, and the error between the tilted angle
of microstructures and laser incident angle was within 2°. The unscanned area
affected the fabrication of the tilted microstructures, where a width of 80–100 µm was
found to be the most suitable for the unscanned area. The height of the
microstructures was greatly increased by increasing the laser output power and
scanning times. However, a laser incident angle 60°, a laser output power of 27 W, 30
scanning times, and an unscanned area width of 100 µm were the most suitable and
economic machining parameters for fabricating the dry metal electrodes with 60°
tilted microstructures. In addition, the dry metal electrodes with tilted microstructures
had much smaller impedance in a bioelectrical measurement compared with those
with vertical microstructures. Therefore, the developed dry metal electrodes with
tilted microstructures, which are economic and convenient, have promising
applications in bioelectrical measurement.
Page 14 of 21
This work was supported by the National Natural Science Foundation of China (Project
No. 51475397) and the Fundamental Research Funds for Central Universities, Xiamen
University (Project No. 20720160079). In addition, the supports from Open Fund of
Shanghai Key Laboratory of Digital Manufacture for Thin-Walled Structures
(No.2015004) and the Collaborative Innovation Center of High-End Equipment
Wei Zhou received received his Ph.D. degrees in mechanical engineering from South
China University of Technology, Guangzhou, China,in 2010. From 2010 to 2012, he
was a postdoc researcher at Sun Yat-sen University. He was appointed as an associate
professor in mechanical & electrical engineering of Xiamen University from Dec 2012
- Juy 2016. Now he is an professor at Xiamen University. His current research interests
focus on design, fabrication and performance evaluation of biomedical device.
Shaoyu Liu starts to work toward the Ph.D. degree in mechanical engineering at
Xiamen University 2014. His research interests are in microfabrication technology of
Wei liu starts to work toward the Ph.D. degree in mechanical engineering at
Xiamen University since 2014. Her research interests are in the area of measurement
methods of different bioelectrodes.
Chenying Zhang starts to work toward the Ph.D. degree in mechanical engineering at
Xiamen University since 2014. His research interests are in the area of the
optimization of fabrication process of bioelectrodes.
Yaoyao Li starts to work toward the M.D. degree in mechanical engineering at
Xiamen University since 2017. His research interests are in the area of the design and
fabrication method of bioelectrodes.
Wenjing Xu starts to work toward the M.D. degree in mechanical engineering at
Xiamen University since 2014. Her research interests are in the area of modeling and
s i m u l a t i o n
of microfabrication process of bioelectrode.
Kwan San Hui received his PhD degree in the department of mechanical engineering
at the Hong Kong University of Science and Technology in 2008. He was appointed as
Page 15 of 21
a lecturer in department of systems engineering and engineering management of City
University of Hong Kong, Hong Kong from Aug 2008 - Feb 2012. In Mar 2013, he
worked as an Assistant Professor in Department of Mechanical Engineering at Hanyang
University, South Korea. In Sep 2016, he was appointed as a Lecturer in Mechanical
Engineering, School of Mathematics, Faculty of Science, University of East Anglia,
UK. He has extensive research experience in material science, catalysis, air/water
p o l l u t i o n
control, and energy storage.
Manufacturing in Fu Jian are also acknowledged.
 S. Enrique, H. Marcelo, Insulating electrodes: A review on biopotential front ends
for dielectric skin-electrode interfaces, Physiol. Meas. 31(2010) 183-198.
 L. S. Hsu, S.W. Tung, C.H. Kuo, Y. J. Yang, Developing barbed microtip-based
electrode arrays for biopotential measurement, Sensors. 14 (2014) 12370–12386.
 S.J. Lee, H.S. Hoon, X. Xuan, J.Y. Park, A patch type non-enzymatic biosensor
based on 3D SUS micro-needle electrode array for minimally invasive continuous
glucose monitoring, Sens. Actuators, B. 222 (2016) 1144–1151.
 P. Griss, P. Enoksson, H. K. Tolvanen-Laakso, P. Merilainen, S. Ollmar, G.
Stemme, Micromachined electrodes for biopotential measurements, J.
Microelectromech. S. 10 (2001) 10–16.
 P. Griss, P. Enoksson, H. K. Tolvanen-Laakso, P. Merilainen, G. Stemme,
Characterization of micromachined spiked biopotential electrodes, IEEE T. Bio-
med. Eng. 49 (2002) 597–604.
 W.C. Ng, H.L. Seet, K.S. Lee, N. Ning, W.X. Tai, M. Sutedia, J.Y.H. Fuh, X.P. Li,
Micro-spike EEG electrode and the vacuum-casting technology for mass
production, J. Mater. Process. Technol. 209(2009) 4434–4438.
Page 16 of 21
 P. Salvo, R. Raedt, E. Carrette, D. Schaubroeck, J. Vanfleteren, L. Cardon, A 3D
printed dry electrode for ECG EEG recording, Sens. Actuators, A. 174 (2012) 96–
 G. Ruffini, S. Dunne, E. Farres, J. Marco-Pallares, C. Ray, E. Mendoza, R. Silva,
C. Grau, A dry electrophysiology electrode using CNT arrays, Sens. Actuators, A.
132 (2006) 34–41.
 N. Kitamura, J. Chim, N. Miki, Electrotactile display using microfabricated micro-
needle array, J. Micromech. Microeng. 25 (2015) 025016.
 M. Tezuka, N. Kitamura, K. Tanaka, N. Miki, Presentation of various tactile
sensations using micro-needle electrotactile display, PLoS One. 11 (2016)
 R. Prehn, M. Cortina-Puig, F.X. Mun, A non-enzymatic glucose sensor based on
the use of gold micropillar array electrodes, J. Electrochem. Soc. 159 (2012) 134–
 Y. Wang, W.H. Pei, K. Guo, Q. Gui, X.Q. Li, H.D. Chen, J.H. Yang, Dry electrode
for the measurement of biopotential signals, Sci. China Inform. Sci. 54 (2011)
 C.F. Pan, K.Y. Chen, L.L. Jiang, Z.P. Chen, L. Ren, L. Liang, W. Yuan,
Magnetization-induced self-assembly method: Micro-needle array fabrication, J.
Mater. Process. Technol. 227 (2016) 251–258.
 M. Tang, V. Shim, Z. Y. Pan, Y. S. Choo, M. H. Hong, Laser ablation of metal
substrates for super-hydrophobic effect, J. Laser Micro. Nanoen. 6 (2011) 6-9.
Page 17 of 21
 Y. C. Guan, W. Zhou, Z. L. Li, H. Y. Zheng, G. C. Lim, M. H. Hong, Femtosecond
laser-induced ripple structures on magnesium. Appl. Phys. A Mater. Sci. Process.
115 (2014) 13-18.
 H. S. Gill, M.R. Prausnitz, Coated microneedles for transdermal delivery, J.
Control. Release. 117(2007) 227-237.
 W. Zhou, R. Song, X.L. Pan, Y.J. Peng, X.Y. Qi, J.H. Peng, K.S. Hui, K.N. Hui,
Fabrication and impedance measurement of novel metal dry bioelectrode, Sens.
Actuators A. 201 (2013) 127–133.
 S.W. Lee, H.S. Shin, C.N. Chu, Fabrication of micro-pin array with high aspect
ratio on stainless steel using nanosecond laser beam machining, Appl. Surf. Sci.
264 (2013) 653–663.
 X. Wang, L.Y. Li, Z.B. Shen, C.F. Sha, Experimental investigation on: Laser shock
micro-forming process using the mask and flexible pad, Opt. Lasers Eng. 88 (2017)
 L. M. Vilhena, M. Sedlacek, Surface texturing by pulsed Nd:YAG laser, Tribol.
Int. 42 (2009) 1496–1504.
 M. Miyagi, X.D. Zhang, Y. Kawahito, S. Katayama, Surface void suppression for
pure copper by high-speed laser scanner welding, J. Mater. Process. Technol. 240
 A. K. Srivastava, B. Bhartia, K. Mukhopadhyay, A. Sharma, Long term
biopotential recording by body conformable photolithography fabricated low cost
polymeric microneedle arrays, Sens. Actuators A. 236 (2015) 164–172.
Page 18 of 21
 L. Chinteng, L. Lunde, L. Yuhang, B.S. Lin, J.Y. Chang, Novel dry polymer foam
electrodes for long-term EEG measurement, IEEE T. Bio-med. Eng. 58(2011)
 T. Gratieri, I. Alberti, M. Lapteva, Y.N. Kalia, Next generation intra- and
transdermal therapeutic systems: Using non- and minimally-invasive technologies
to increase drug delivery into and across the skin, Eur. J. Pharm. Sci. 50 (2013)
 J. H. Park, S. O. Choi, S. Seo, Y. Bin Choy, M. R. Prausnitz, A microneedle roller
for transdermal drug delivery, Eur. J. Pharm. Biopharm. 76 (2010) 282–289.
 S. A. Ranamukhaarachchi, T. Schneider, Development and Validation of an
Artificial Mechanical Skin Model for the Study of Interactions between Skin and
Microneedles Macromol. Mater. Eng. 301(2016) 306−314.
 M. Arai1, Y. Nishinaka, Electroencephalogram measurement using polymer-based
dry microneedle electrode, Jpn. J. Appl. Phys. 6 (2015) 06FP14.
 B. H. Brown, Medical impedance tomography and process impedance
tomography: a brief review. Meas. Sci. Technol. 12(2001) 991–996.
 J. Ho, C. Grigoropoulos, J. Humphrey, Computational study of heat-transfer and
gas-dynamics in the pulsed-laser evaporation of metals, J. Appl. Phys. 78(1995)
 L. M. Vilhena, M. Sedlacek, Surface texturing by pulsed Nd:YAG laser, Tribol.
Int. 42 (2009) 1496–1504.
 D. Du, Y.F. He, B. Sui, L.J. Xiong, H. Zhang, Laser texturing of rollers by pulsed
Page 19 of 21
Nd:YAG laser, J. Mater. Process. Technol. 161(2005) 456–61.
Fig.1 Schematic diagram of dry metal electrode with tilted microstructure array：1-
metal electrode core, 2-shielding wire, 3-conductive silver glue, 4-foam backing
material, and 5- medical gauze
Fig.2 Schematic diagram of the experimental setup for the laser micromilling process
used for the dry metal bioelectrode.
Fig.3 Schematic diagram of impedance measurement of dry metal electrode
Fig.4 Schematic diagram of forming process of tilted microstructure array on the dry
Fig.5 Typical SEM image of a tilted microstructure array on the surface of a dry metal
Fig.6 SEM images of dry metal electrodes with tilted microstructure arrays fabricated
with different laser incident angles：(a) 60°, (b) 70°, (c) 80°, and (d) 90°（Vertical
Fig.7 SEM images of dry metal electrodes with tilted microstructure arrays fabricated
with different unscanned area widths：(a) 60 µm, (b) 80 µm, (c) 100 µm, and (d) 120
Fig.8 influence of the unscanned area width on the height and bottom width of tilted
microstructurethe of dry metal electrode
Fig.9 SEM images of dry metal electrodes with tilted microstructure arrays fabricated
with different laser output power values: (a) 21 W, (b) 24 W, (c) 27 W, and (d) 30 W
Page 20 of 21
Fig.10 Influence of laser output power on height and bottom width of tilted
microstructures of dry metal electrode
Fig.11 SEM images of dry metal electrodes with tilted microstructure arrays fabricated
with different scanning times：(a) 10, (b) 20, (c) 30 and (d) 50
Fig.12 Influence of scanning times on height and bottom width of tilted microstructures
of dry metal electrode
Fig.13 Impedance measured value using dry metal electrodes with different tilted
degree microstructure array and without microstructure array
Table 1 Specifications of characteristic parameters of fiber laser system
Table 2 Tilted angle and height of microstructures fabricated with different laser
Page 23 of 21
Page 24 of 21
Laser output power（ W）
Page 25 of 21
Page 26 of 21
Page 27 of 21
(a) Average impedance over 20
(b) Impedance measurement over 20 min
Page 28 of 21
Page 29 of 21
Dry electrodes LCR
Page 30 of 21
Side length of unscanning area
Bottom width of microstructure
Page 31 of 21
Page 32 of 21
Page 33 of 21
Page 34 of 21
60 80 100 120
Width of unscanned area(m)
Page 35 of 21
Page 36 of 21
Characteristic Parameter range Assumed parameter Unit
Wavelength 1055~1070 1064 nm
Nominal average output power
29~31 30 W
Pulse duration 90~120 100 ns
Repetition rate 20~200 20 kHz
Beam quality (M2) <1.1 1
Incident beam diameter 6~9 7 mm
Focused diameter 24.3~37.3 31.5 m
Page 37 of 21
Laser incident angle Height of microstructure (μm) Titled angle of microstructure
60° 459.9 58.3°
70° 395.5 71.8°
80° 371.2 78.2°
90° 320.6 89.5°